CORROSION AND MASS TRANSFER CHARACTERISTICS OF NaBF4-NaF (92-8 mole I N HASTELLOY N J. W . Koger
THIS DOCUMENT CONFtRMED' AS UNCLASSIFIED DIVISION OF CLAsStFiCATION BY qfl&I&w& DATE ' 1611g1d7c '
This report was prepared as an account of work sponsored by the United States Government. Neither the United States nor the United States Atomic Energy Commission, nor any of their employees, nor any of their contractors, subcontractors, or their employees, makes any warranty, express or implied, or assumes any legal liability or responsibility for the accuracy, completeness or usefulness of any information, apparatus, product or process disclosed, or represents that i t s use would not infringe privately owned rights.
Contract No. W-7405-eng-26 METALS AND CERAMICS DIVISION
CORROSION AND MASS TRANSFER CHARACTERISTICS OF NaBFb-NaF (92-8 mole %) IN HASTELLOY N
J. W. Koger NOTICE This report was prepared as an account of work sponsored by the United States Government. Neither t h e United States nor the United States Atomic Energy Commission, nor any of their employees, nor any of their contractors, subcontractors, or their employees. makes any warranty, express or implied, or assumes any legal liability or responsibility for the accuracy, completeness or usefulness of any information, apparatus, product or process disclosed, or represents that its use would not infringe privately owned rights.
NOTICE This document contains information of a preliminary nature and was prepared primarily f o r internal use a t t h e Oak Ridge National Laboratory. I t is subject to revision or correction and therefore does not represent a final report.
OAK RIDGE NATIONAL LABORATORY
Oak Ridge, Tennessee 37830 operated by UNION CARBIDE CORPORATION for the U.S. ATOMIC ENERGY COMMISSION
.............................. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . Experimental Procedure . . . . . . . . . . . . . . . . . . . . . . . Equipment . . . . . . . . . . . . . . . . . . . . . . . . . . .
........................... Operation and Results . . . . . . . . . . . . . . . . . . . . . . . Analyses
Thermal Convection Loops NCL.13.
.......................... LoopNCL.20 .......................... FCL-1 Pump Loop . . . . . . . . . . . . . . . . . . . . . . . . Runsland2 . . . . . . . . . . . . . . . . . . . . . . . Run3 . . . . . . . . . . . . . . . . . . . . . . . . . .
... Run4 . . . . . . . . . . . . . . . . . . . . . . . . . . Run5 . . . . . . . . . . . . . . . . . . . . . . . . . . Run6 . . . . . . . . . . . . . . . . . . . . . . . . . . Run7 . . . . . . . . . . . . . . . . . . . . . . . . . . Salt Chemistry . . . . . . . . . . . . . . . . . . . . . . . . . . . Purification . . . . . . . . . . . . . . . . . . . . . . . . . Installation and Testing of Cold Finger During Run 3
............................. Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . Kinetics . . . . . . . . . . . . . . . . . . . . . . . . . . . Solid-state Diffusion Control . . . . . . . . . . . . . . Solution Controlling . . . . . . . . . . . . . . . . . . . Experimental Data . . . . . . . . . . . . . . . . . . . . Diffusion Calculations . . . . . . . . . . . . . . . . . . . . Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . Acknowledgment . . . . . . . . . . . . . . . . . . . . . . . . . . .
Page . 1 1 6 6 8 11
11 11 20 27 28 32 37 38
40 42 45 48 53 53 54 54
54 61 62 66 67 68 70 76 78 79
CORROSION AND MASS TRANSFER CHARACTERISTICS OF NaBFb-NaF (92-8 mole %) IN HASTELLOY N
J. W. Koger ABSTRACT A series of corrosion experiments in thermal convection and pump loops designed to test the compatibility of fused NaBF44 mole % NaF with Hastelloy N has shown the extreme effect of impurities on the system mass transfer. The difficulty in keeping the melt sufficiently pure was also illustrated. Kinetic considerations showed that the mass transfer process is controlled either by solid-state diffusion or by the solution rate, depending on the amount of impurities allowed to enter the salt. The mass transfer behavior is very similar to that for the Cr-UF4 corrosion'reaction (material removal in the hot section and deposition in the cold section), the differences being that alloy constituents other than chromium participate in the process and that the reaction rates are different. Because of these differences, the effective diffusion rate controlling the hot leg attack is larger-thanthat obtained in typical diffusion experiments for chromium in Hastelloy N.
Titanium-modified Hastelloy N with less chromium and iron shows a greater resistance to attack in a fluoroborate salt with 500 ppm oxide impurity than does standard Hastelloy N. Its corrosion rate is doubled by increasing the oxide concentration to'1500 ppm. Average corrosion rates were low for all systems tested.
INTRODUCTION The successful development and operation of the molten salt reactor experiment (MSW) have led t o the present program for development of a molten salt breeder reactor (MSBR). In the MSRE the heat transferred
from the fuel salt to the coolant salt was rejected to an air-cooled radiator. In the MSBR a secondary coolant will be required to remove heat from the fuel in the primary heat exchanger and transport this heat to supercritical steam at quite low temperatures.
This secondary coolant should have low viscosity and density and high heat capacity and thermal conductivity to permit use of acceptable heat exchangers, coolant pumps, and steam generators. The melting point must be low enough to meet the heat transfer temperature requirements, and the vapor pressure must be low at the temperature of operation. The salt must also be easily remelted, with no precipitation of high-melting compounds during cooling. The coolant must be commercially available in high purity, and the price should not be prohibitive. In nuclear systems the coolant must be stable under the radiation that it encounters. We also must consider the result of accidental mixing of the coolant fluid and steam and select a coolant in which the effects of this mixing will be minimized. Last but not least, the coolant must be compatible with the container materials of the system. It now appears that the best choice for the MSBR secondary coolant is the eutectic mixture of 8 mole % NaF in NaBF4, with a melting point’ of 385°C (725°F) as shown in Fig. 1. The salt is quite inexpensive ’C. J. Barton, L. V. Gilpatrick, H. Insley, and T. N. McVay, MSR Program Semknn. Progr. R e p t . Feb. 29, 1968, ORNL-4254, p. 166. ORNL-DWG 67- 9423A
700 600 500
300 200 NaF
40 60 NaBF4 (mole % 1
Fig. 1. The System NaF-NaBF4.
At elevated temperatures the fluoroborates show an appreciable equilibrium pressure of gaseous BF3; however, at the proposed maximum temperature of the MSBR secondary coolant (621OC) the pressure is only 252 torr. The equilibrium pressure2 above a melt of NaBF4-8 mole % NaF is given as a function of temperature by
9.024 - 5920/T(OK)
Table 1 contains some of the pertinent physical properties for this mixture at temperatures of interest. Other possibilities for secondary coolants, such as fluorides, chlorides , and liquid metals, are discussed elsewhere.
Before our compatibility tests4, with the sodium fluoro-
borate mixture, little was known or reported about its corrosive behavior in the molten state. Because of its appreciable vapor pressure at temperatures of interest, BF3 corrosion is of importance also. In corrosion experiments6 with gaseous BF3, it was rapidly attacked by traces of moisture to give hydroxyfluoboric acid (HBF3OH) and HF. Also BF3 and glass reacted at an-appreciablerate just above 200OC. Under the conditions of those experiments, BF3 did not appreciably attack a wide variety of metals or alloys examined at temperatures up to 200OC. 2S. Cantor, J. W. Cooke, A. S. Dworkin, G. D. Robbins, R. E. Thoma, and G. M. Watson, PhysicaZ Properties of Molten Salt Reactor Fuel, ORNL-TM-2316 (August 1968).
3W. R. Grimes, "Molten-Salt Reactor Chemistry," NucZ. AppZ. TechnoZ. 142 (1970). 4J. W. Koger and A. P. Litman, Compatibility of HasteZZoy N and Croloy 9M with NaBF4-NaF-KBF4 (90-4-6 mole X) FZuoroborate Salt, OW-TM-2490 (April 1969). 8:
.5J. W. Koger and A. P. Litman, Compatibility of 'Fused Sodium-. Fluoroborates and BF3 Gas with Hastelloy N Alloys, ORNL-TM-2978 . (June 1970). 6F. Hudswell, J. S. Nairn, and K. L. Wilkinson, "Corrosion Experiments with Gaseous Boron Trifluoride," J. AppZ. Chem. 1: 33336 (1951).
4 Some Properties of the Mixture NaBF4-8 mole X NaF
Approximate melting point, OC Vapor pressure at 621째C, torr Density, at at at at
TOC 621OC 538OC 455OC
1.82 1.87 1.93
Viscosity,b centipoise: rl = 0.0877 exp(2240/T)
at T O K at 621OC at 538OC at 455OC Heat Capacity:
1.1 1.4 1.9 C
c = 0.360 cal 8-l OC-' P d Thermal Conductivity: at 621OC:K = 0.0039 W em-' OC-l at 538"C:K = 0.0041 W cm" OC-' at 455"C:K = 0.0043 W cm-' OC-' Latent Heat of Fusion = 31 cal/g a
S. Cantor, MSR Program S e m k n n . Progr. Rept. Aug. 31, 1969, ORNL-4449, p. 14.
bS. Cantor, MSR Program S e m b n . Progr. Rept. Aug. 31, 1969, ORNL-4449, p. 145. C
A. S. Dworkin, MSR Program Semiann. Progr. Rept. Feb. 29, 1968, ORNL-4254, p. 168. dJ. W. Cooke, MSR Program Semiann. Progr. Rept. Aug. 31, 19169, ORNL-4449, p. .92.
Ld I I
All metal components of the MSRE in contact with molten salt were made of Hastelloy' N (formerly called INOR-8). Two decades of corrosion testing8-' and experience16-19 with the MSRE have demonstrated the excellent compatibility of Hastelloy N and graphite with fluoride salts containing LiF, BeF2, UF4, and ThF4. Hastelloy N, perhaps with some modification of composition, is quite likely to be the primary containment material for MSBR. Thus, it was of great interest to the molten salt program to determine the compatibility of the fluoroborate salt mixture with Hastelloy N and related alloys. Of special interest is temperature-gradient mass transfer, which must always be considered where corrosion in a heat exchanger is possible. Corrosion and deposition processes'in flowing nonisothermal systems are interdependent, and each exerts considerable influence over the extent and characteristics of the other. Therefore, a performance analysis of a nonisothermal system must consider these processes as complementary and equal in significance to the overall system behavior, This paper is an up-to-date, open-ended report on these studies.
Hastelloy N is the traae name of Cabot Corporation for a nickelbase ailoy containing 16% Mo, 7% Cr, 5% Fe, and 0.057% C. 8 L. S, Richardson, D. C. Vreeland, and W. D. Manly, Corrosion by Molten Fluorides: Interim Report for September 1952, ORNL-1491 (April 20, 1953). , 9
G. M. Adamson, R. S. Crouse, and W. D. Manly, Interim Report on Corrosion b y AZkaZi-MetaZ FZuorides: Work t o May I, 1953, ORNL-2337 (March 20, 1959). 'OG. M. Adamson, R. S. Crouse, and W. D. Manly, Interim Report on Corrosion by Zirconium-Base Fluorides, ORNL-2338 (Jan. 3, 1961). "W. B. Cottrell, T. E. Crabtree, A. L. David, and W. G. Piper, DisassembZy and Postoperative Examination of the Aircraft Reactor Experiment, OW-1868 (April 2, 1958). 12 W. D. Manly, G. M. Adamson, Jr., J. H. Coobs, J. H. DeVan, D. A. Douglas, E. E. Hoffman, and P. Patriarca, Aircraft Reactor E@er$ment-MetuZZurgicaZ Aspects, ORNL-2349, pp 2-24 (Dec. .20,1957) 13 W. D. Manly, J. H. Coobs, J. H. DeVan, D. A. Douglas, H. houye, P. Patriarca, T. K. Roche, and J. L, Scott, "Metallurgical Problems in Molten Fluoride Systems," Progr. Nucl. Energy Ser. I V 2: 164-79 (1960). i
i ! i 1
EXPERIMENTAL PROCEDURE Equipment In corrosion studies the thermal convection loop represents an intermediate stage of sophistication and complexity between simple capsule tests and a full-scale engineering pump loop experiment. It is particularly suited to small-scale tests that involve temperaturegradient mass transfer. The flow of the liquid is caused by its variation in density with temperature. The development of a modified thermal convection loop has permitted important strides in obtaining basic corrosion information. The thermal convection loop used in this work and shown in Fig. 2 permits unrestricted access to specimens and salt at any time without significantly disturbing loop operation or introducing air contamination.
Access is provided by twin ball valve arrangements
atop both the hot and cold legs of the loops. The molten salt sampling device illustrated in Fig. 3 was used in our thermal loops and can also 14
W. D. Manly, J. W. Allen, W. H. Cook, J. H. DeVan, D. A. Douglas, H. Inouye, D. H. Jansen, P. Patriarca, T. K. Roche, G . M. Slaughter, A. Taboada, and G. M. Tolson, Fluid Fuel Reactors, pp. 595-604, James A. Lane, H. G. MacPherson and F. Maslan, eds., Addison Wesley, Reading, Pa., 1958. "J. H. DeVan and R. B. Evans 111, "Radiotracer Techniques in the Study of Corrosion by Molten Fluorides," pp. 557-79 in Conference on Corrosion of Reactor Materials, June 4 4 , 1962, Proceedings VoZ. 11, International Atomic Energy Agency, Vienna, 1962. 16H. E. McCoy, An Evaluation of the Molten-Salt Reactor Experiment Hastelloy N Surveillance Specimens - First Group, ORNL-TM-1997 (November 1967). 17H. E. McCoy, An Evaluation of the Molten-Salt Reactor Experiment Hastelloy N Surveillance Specimens - Second Group, ORNL-TM-2359 (February 1969). '%.E. McCoy, An Evaluation of the Molten-Salt Reactor Experiment HasteZloy N SurveiZZance Specimens - Third Group, ORNL-TM-2647 (January 1970). \ "H. E. McCoy, An Evaluation of the Molten-SaZt Reactor Expkriment HasteZZoy N Surveillance Specimens - Fourth Group, ORNL-TM-3063 (March 1971).
F CORROSION SPECIMENS-
F i g . 2.
MSRP Natural Circulation Loop and Salt Sampler.
8 ORNL-DWG 68-2796
Molten Salt Sampling Device.
be used in pumped loops. Typical thermal convection loops in operation are shown in Fig. 4. A forced convection loop was also used to evaluate the fluoroborate
salt mixture and will be described later. Salt Preparation The salt for these tests was processed by the Fluoride Processing Group of the Reactor Cbemistry Division. Very pure (> 99.9%) starting materials were evacuated to about 380 torr, heated to 150째C in a vessel lined with nickel, and then held for about 15 hr under these conditions.
Thermal Convection Loops in Operation.
10 If the rise in pressure was not excessive (indicating no volatile impurities), the salt was heated to 500째C while still under vacuum and agitated for a few hours with bubbling helium. It was then transferred to the fill vessel and from it forced into the loops with helium pressure. In the case of the pumped loop the salt was transferred initially into a dump
tank and then into the loop tubing. The hot portion of each thermal convection loop was heated by sets of clamshell heaters, with the input power controlled by silicon controlled rectifiers (SCR units) and the temperature controlled by a Leeds and Northrup Speedomax H series 60 type CAT controller. The loop temperatures were measured by Chromel-P vs Alumel thermocouples spot welded to the outside of the tubing, covered first by quartz tape and then by stainless steel shim stock. Each loop was degreased with ethyl alcohol, heated to 150째C under vacuum to remove moisture, and leak checked before filling with salt. All lines from the fill tank to the loop that were exposed to the fluoroborate salt were of the same material as the loop and were cleaned and tested in the same manner as the loop. All temporary line connections were made with stainless steel compression fittings. Each loop was filled by heating it, the salt pot, and all connecting lines to at least 53OOC and applying helium pressure to the salt pot to force the salt into the loop. Air was continuously blown on the freeze valves leading to the dump and flush tanks to provide a positive salt seal. Tubular electric heaters controlled by variable autotransformers heated the cold-leg portions. Once the loop was filled the heaters were turned off, and the proper temperature difference was obtained by removing some insulation to,exposeportions of the cold leg to ambient air. The-firstcharge of salt was circulated under a small temperature difference (2OOC) for 24 hr and dumped. This flush removed surface oxides and other possible impurities. The loops were then refilled with new salt and put into operation. A helium cover gas under slight positive pressure (about 5 psig) was maintained over the salt in the loops during operation.
Analyses Several methods can be used to obtain quantitative data from a temperature-gradient mass transfer exper$ment relating to the kinetics
of mass transfer, the thermodynamics.of the process, or both. The most obvious and easiest to obtain are weight change measurements on specimens and liquid analyses. The weight changes allow the calculation of mass transfer rates in both legs, We may also analyze specimens and loop tubing with a microprobe to determine composition gradients, x-ray fluorescence to determine the surface composition, and spectrochemistry to determine overall composi.tion. Standard metallographic examination is also helpful to determine the extent of attack or void formation in the hot leg or the amount of deposit in the cold leg. OPERATION AND RESULTS The:results of tests of the fluoroborate salt mixture in two thermal convection lbops and in a series of capsule tests have already been Leported-.2 o s2'
In addition, four other thermal convection loops and one
pumped loop have been operated.
These latter tests are described below,
'and-results'of all the tests are reviewed. .
Thermal Convection Loops NCL-13, NCL-l3A, and NCL-14
Thermal convection loops NCL-13,:and NCL-14 (constructed of standard
Hastelloy N) were started at the same time under the .identicalconditions of 605째C maximum temperature and a temperature difference of 145OC. These operating conditions were those proposed for the coolant circuit of the MSRE. During circulation each loop (0.75-in.-OD X 0.072-in.-wall tubing) contained about 2.7 kg of salt that contacted 1740 cm2 (270 in.2)
2oJ. W, Koger and A. P. Litman, Compatibility of Hastelloy N and Croloy 9M with N~BFI,-N~F-KBFI,' '(90-4-6 mole X) Fluoroborate Salt, OWL-TM-2490 (April 1969). 21J, W. Koger and A. P.'Litman, Compatibility of Fused Sodium Fluoroborates and BF3 Cas with Hastelloy N Alloys, ORNL-TM-2978 (June 1970).
of surface and traveled 254 cm around the harp. Typical flow under the above conditions was 7 ft/min. Loop NCL-13 contained standard Hastelloy N specimens, while loop NCL-14 had titanium-modified Hastelloy N suspended in the salt stream. The compositions of these alloys are given in
Table 2. The modified alloy is being considered because of its superior mechanical properties under radiation at elevated temperature. Table 2. Composition of Hastelloy N Alloys
Alloy Standard Hastelloy N
Content, wt X Ni
Titanium-modified Hastelloy N 78
0.6 0.54' 0.02
0.01 0.14 0.5
The weight changes measured for the specimens in NCL-13 and NCL-14 showed an increase in mass transfer rate between 3500 and 4300 hr of exposure to the salt (Fig. 5 ) . This was accompanied by perturbations in I
salt composition. Analyses of the circulating salts from these loops showed that the oxide content increased to above 2000 ppm (from initially less than 1000 pprn), and the nickel and molybdenum contents exceeded 100 ppm (from below 25 ppm). Also, the chromium and iron contents
increased "normally" with time, as shown in Fig. 6 . After 4700 hr of operation, the helium gas regulator that provided the overpressure to NCL-13 failed and caused a surge bf gas to the loop, stopping the salt flow. Circulation of the salt could not be resumed until a vacuum was pulled on the loop, which we believe removed a gas pocket.
Shortly after circulation was restored, an electrical short,
which eventually burned out a heater, occurred and heated the bottom of I I
the hot leg to 870째C (1600'F). This disrupted the flow and caused a loss of BF3 from the loop, which changed the salt composition and plugged all the gas lines. The loop was drained' of all salt, and plugged lines were replaced or unplugged.
Other necessary repairs to the loop were made, and the loop was filled with new salt. The loop was then designated as NCL-13A.
l ORNL- DWG 68- 13717
/ HOTTEST SPECIMENS
607 O C
TITANIUM MODIFIED HASTELLOY N-NCL-44 STANDARD HASTELLOY
3 4 TIME (hr)
Fig. 5. Weight Change Versus Time for Standard and Titanium-Modified Hastelloy N Specimens in NCL-13 and NCL-14 Exposed to Fluoroborate Salt at Various Temperatures.
Fig. 6. Average Concentrations of Iron and Chromium in the Fluoroborate Salt in NCL-13 and NCL-14.
14 After new fluoroborate salt was gdded to loop NCL-l3A, circulation could not be achieved. We concluded that previous overheating of the loop had caused BF3 to evolve and had made the salt much richer in NaF. This in turn caused the higher melting NaF to segregate in the loop. To bring the composition back to normal, we added BF3 gas to the melt through the surge tank. The initial amounts of gas were dissolved in the salt, and additions continued until a slight overpressure built up over the salt. (No devices were available to measure the amount of BF3 gas added.) Circulation of the salt was then attempted and was successful. Only a small temperature difference (55OC) was obtained at first. Further additions of BF3 as before lowered the temperature of the salt in the cold leg and increased the temperature difference to about 125OC.
BF3 did not cause immediate changes and did not appear to dissolve in the salt, the additions of gas were stopped. The loop has since operated satisfactorily. Loops NCL-13A and NCL-14 have now operated for two and three years, respectively. Figure 7 gives the weight changes of specimens at various temperatures as functions of operating time. The overall corrosion rates at the maximum temperature, 605OC, are 0.5 and 0.7 mil/year for loops NCL-13A and NCL-14, respectively. The attack is general, and actual measurements of specimens show changes in thickness agreeing with those calculated from weight changes. We will now discuss the circumstances that have affected the mass transfer conditions. The air leaks in loops NCL-13A and NCL-14 occurred at various mechanical joints in the system, such as ball valves, level probes, and pressure gages, all located in the cover gas space above the circulating salt. We had gained extensive experience with similar mechanical joints before testing fluoroborate salt mixtures and had encountered no leakage problems. Therefore, the frequency of leaks in these two fluoroborate loops strongly suggests that the BF3 atmosphere in these tests has deteriorated our mechanical seals. We are currently investigating the chemical nature of the BF3 to determine any possible contaminants which might have caused such deterioration. Despite the known problems of air leakage, these loops have operated for over two years with the fluoroborate salt, and the overall corrosion rate is within acceptable limits. I
ORNL-DWG 69- 47638
I 12 W
-30 - 40 - 50 1
TIME OF OPERATION (hr)
Fig. 7. Weight Change Versus Time for Standard Hastelloy N Specimens in NCL-13A and Titanium-Modified Hastelloy N Specimens in NCL-14 Exposed to Fluoroborate Salt at Various Temperatures.
16 We also used loop NCL-14 to determine the corrosion properties of pure Cr, Fe, Mo, and Nickel 280 (commercially pure nickel with A1203 added as a grain refiner) at 6OO0C in the fluoroborate mixture. As a consequence of the air leaks discussed above, the oxide content of the salt in loop NCL-14 was at an abnormally high level and indicated fairly strongly oxidizing conditions. We initially examined the pure metal specimens after a 234-hr exposure. On removal, we found that the chromium and iron specimens had completely disintegrated. The molybdenum specimen showed no weight change, and the nickel specimen showed a slight weight gain. The chromium and iron specimens were replaced, and a second experiment was conducted for 23 hr. Again, the molybdenum specimen did not change weight, and the nickel specimen showed a slight weight gain. Very little of the chromium specimen remained, and the Close weight loss of the iron specimen was 40 mg/cm2 (70 mils/year). examination of the chromium specimen showed it to be coated with a black reaction layer about 0.015 in. thick. Laser spectroscopy of the outer surface of the black material showed iron and boron as major constituents and sodium and chromium as minor constituents. However, x-ray diffraction of the bulk coating showed it to be over 90% NaBF4. This black coating has been observed on Hastelloy N specimens exposed to impure NaBF4-8 mole % NaF in the past,22 but in these cases it was too thin or too adherent to remove and identify. Attack of Hastelloy N by impure fluoroborate salt tends to be nonselective; that is, all components of Hastelloy N suffer oxidation, and surfaces of the alloy appear to recede uniformly.
However, in this experiment with pure metals, only the chromium and iron were noticeably
attacked, the chromium more than iron. We conclude, therefore, that the pure chromium and iron specimens in this system inhibited the attack of the nickel and molybdenum specimens. The inhibition apparently is much less when chromium and iron are present as alloying additions in Hastelloy N, presumably because their chemical activity in the alloy is too low or the rate at which they can enter the salt is too slow, being limited by solid-state diffusion in the alloy. When the 22J. W. Koger and A. P. Litman, MSR Program Semfann. Progr. R e p t . Feb. 29, 1968, ORNL-4254, p . 225,
17 oxidation pbtential of the salt is reducFd, owever,; as-wouldbe the case in a purer fluoroborate s.al selective, and the buffering effect of chromi [
tant. In loop tests of nickel-molybde alloys containing Fe, Nb, or W, DeVan observed2 that the concentra of these elements in FLINAK24 salt was lowered by the presence of chromium in the alloy. These observations suggest that the incorporation of an active metal such as chromium would effectively inhibit attack in a Hastelloy N4luoroborate circuit. Figure 8 shows optical and scanning electron micrographs of specimens from the hot and cold leg of NCL-13. These specimens were exposed to NaBF4-8 mole % NaF for 4180 hr at 580 and 476OC. The hot-leg specimen lost 3.3 mg/cm2, and the cold-leg specimen gained 3.2 mg/cm2. The surface of the hot-leg specimen, as seen in Fig. 8 (left) has been attacked nonuniformly and is heavily contoured. Figure 8 (right) shows that the cold-leg specimen is coated with a discontinuous deposit, which is essentially analyzed as Hastelloy N slightly enriched in nickel and molybdenum. The dumped salt from NCL-13 was chemically analyzed, and the results The Cr, Fe, Ni, Mo, 0, and H20 contents of the salt all showed large increases. Increases in the nickel and molybdenum
are given in Table 3.
content of the salt often indicate the onset of stronger oxidizing conditions, usually due to increased water or oxygen content. Thus the most obvious explanation of the composition changes and increased weight changes was contamination by water, which produced HF, which in turn attacked all the constituents of the container material. This was substantiated by the discovery of a faulty helium line common to both loops. This line admitted air. Loop NCL-14 initially operated about 3500 hr with the oxide content in the salt between 500 and 1000 ppm. During that period the weight changes were small and predictable as a function of time, Wet air then
23.T. H. DeVan, Effeat of A l l o y i n g 'Additions on Corrosion Behavior luoride Mixtures, OWL-TM-2021, of Nickel-Molybdenum Alloys in Fuse Vole 1, Pp* 38-39 (May 1969) 24Composition: NaF-LIF-KF-UF4 (11.2-45.3-41.0-2.5 mole %).
Fig. 8. Hastelloy N Specimens from NCL-13 Exposed to NaBF4-8 mole X NaF for 4180 hr. Left: in hot leg at 580OC; weight loss 3.3 mg/cm2. Right: in cold leg at 476째C; weight gain 3.2 mg/em2. Top: optical micrographs at 500X, etched with glyceria regia. Bottom: scanning electron micrographs at 3000X (left) and 1OOOX.
Table 3. Chemical Analyses of Fluoroborate Salt in NCL-13 I
Salt before loop operation Dumped salt circulated for 4700 hr
Content, ppm Fe Ni Mo
Content, wt % Na B F
came in contact with the salt through the defective gas line, and the water content and corrosion rate increased dramatically. During the next 5000 hr the oxide content of the salt decreased, and the corrosion rate again decreased as a function of time. The maximum rate of weight mg cm-2 hr-' loss during this 5000-hr period was about 1.5 x
(0.65 mil/year) This corrosion rate is double that measured during the earlier operating period.
,Theconcentration of impurities in the salt in loop NCL-14 is given as a function of operating time in Fig. 9. The second change in corrosion rate, at some time between 11,000 and 13,000 hr, was due to a leaking standpipe ball valve. This last intake of impurities illustrates a continuing'problem of detection (other than the obvious after-the-fact increase of impurities and corrosion rate), since the loop overpressure did not change'significantly. Apparently moisture from the air effuses into the relatively moisture-free atmosphere of the loop (equalization of partial pressure) without the need for a gradient in overall pressure. In this last corrosion rate increase period the analyzed oxide content of the salt increased from 1300 to 4500 ppm.
The ball valve was repaired,
the loop continued to operate. .and . As we have shown, abrupt increases in the slope of the weight change curves (increased rates of gain and l o s s ) indicated changes in the oxidation potential of the salt, which were caused by inadvertent air leaks into the system. These slope changes were accompanied by increases in Cr, Ni, Fe, and Mo contents in the salt, which would indicate general attack of the alloy. Under conditions where external impurities did not
20 , ORNL-DWG 68-11768AR
250 200 450 400
6000 8000 TIME (hr)
Fig. 9 . Variation of Impurity Contents with Time in NaBF4-8 mole % NaF Thermal Convection Loop NCL-14. enter the loops, chromiumwas the only element removed from the alloy, and corrosion rates during these periods fell to as low as 0.08 mil/year. LOOP NCL-17 Loop NCL-17, constructed of commercial Hastelloy N with removable specimens in each leg, is being operated to determine the effect of steam inleakage in a fluoroborate salt-Hastelloy N circuit. The maximum temperature is 607OC with a temperature difference of 107째C.
This experiment has run for over 10,000 hr and is continuing in order to provide information on the immediate and long-range corrosi.onof the system after steam injection. The loop was operated for 1050 hr, the specimens were removed and weighed, and steam was forced into the flowing salt system through a
16-mil hole in a closed 1/4-in. Hastelloy N tube, simulating a leaking heat exchanger. Steam was forced-intothe system until the pressure of the cover gas began to increase, thus indicating that no more steam was soluble in the salt. Figure 10 shows the weight changes and temperatures for the specimens in NCL-17. As usual, the changes depend on temperature, and the rates decrease with time after an initial rapid rate. The corrosion rate appears to have stabilized, and no plugging conditions have
been noted. Figure 11 shows the specimens from the loop 424 hr after exposure to steam. The specimens with the etched appearance have lost weight, and those that are darkened have gained weight. For the last 3500 hr of operation, as shown in Table 4, the concentrations of impurityâ€™constituentsin the salt (Fe, Cr, Ni, Mo, and 0) remained relatively constant. The present chromium level is abow 320 ppm. The results 0% this test show that the Hastelloy N system
pw -to a I u I-
- 50 c
TIME OF OPERATION (hr)
Fig. 10. Weight Change Versus Time for Hastelloy N Specimens in NCL-17 Exposed to NaBFt,â€™-8 mole % NaF at Various Temperatures.
Fig. 11. Hastelloy N Specimens from NCL-17 Exposed to NaBF44 mole % NaF. Specimens were exposed to salt for 1050 hr before steam injection and for 424 hr after steam injection. The specimens on the left were in the hot leg, and those on the right were in the cold leg. Specimens with the etched appearance lost weight, and the darkened specimens gained weight.
23 ntration of Impuri
in NCL-17 Salt
1180 1182 1468
< 5 Added steam
11 15 11
containing fluoroborate salt can tolerate inleakage of steam and, once the leak is repaired, can continue to operate without extensive damage even if the salt is not repurified. Figure 12 shows micrographs of the specimens in the hottest and coldest positions. The attack seen in the hot leg is general, as expected for impurity-controlled mass transfer processes. Micrometer measurements show a loss of about 1 mil from specimen surfaces at the maximum temperature position.
In Fig. 12(b) we see a large amount (about
2 mils) of deposited material. T h i s material has been analyzed with an electron beam microprobe, and Table 5 gives the results for the substrate and the deposit. These results show that very little chromium has deposited. The nickel and molybdenum concentrations reached maxima of 74 and 56 ppm, respectively, 288 hr after the steam addition, decreased, and quickly leveled off to about 10.ppmeach. From the microprobe evidence much of the nickel and molybdenum apparently deposited in the cold
leg, although not in.the same ratio as they exist in Hastelloy N. .One may conclude that under highly oxidizing conditions, during which large weight changes occur (NCL-J.4 during the air leak and NCL-17 after steam inleakage), most of the changes are attributable to the movement of the
Fig. 12. Microstructure of Standard Hastelloy N Exposed to NaBF4-8 mole % NaF in NCL-17 for 3942 hr. Steam was injected into salt after 1054 hr. (a) 607"C, weight loss 26.8 mg/cm2, as polished; (b) 495OC, weight gain 14.8 mg/cm2, as polished. A relatively spongy surface layer on this sample is about 2 mils thick. 500~.
25 e Analysis of Spec n in Coldest Position Table 5 . Micro (493OC) in LaopvNCL-17 .Exposed to Fluoroborate Salt for 0 hr; Steam Injected into Salt 1000 h eginning of Run Composition Substrate
Cr Fe P Undetermined
wt % Deposit
34.8 30.6 C 0.5
a Corrected for absorption, secondary fluorescence, and atomic number effects. bThin layer close to sample surface. normally stable nickel and molybdenum. Any increased chromium removal from the hot leg is noted only as an increase in the chromium concentration in the salt. The phosphorus found in the deposit was apparently from a phosphate impurity in the steam. Figure 13 shows optical and sc mens from the hot and cold leg of N
electron micrographs of speciimens at 593 and 5OOOC
were exposed to the salt for 1050 hr, and then' was injected oop' for an additional into the loop. The specimens then remained in 9000 hr. The total weight loss of the hot-leg specimen was 40.9 mg/cm2, and the weight gain of the cold leg was 16.0 mg/c left),we see that the surface receded unifo precipitate was left in relief
In Fig. 13 (top although a Widmansggtten
ig. 13 (lower left) 1
Figure' 13 (top right) shows a dark deposit on the cold-leg specimen, and the deposit exhibits a layered structure when viewed from above [Fig. 13 (lower right)]. i,
Fig. 13. Hastelloy N Specimens from NCL-17 Exposed to NaBF4-8 mole % NaF for 10,050 hr (1050 hr before Steam Addition). Left: in hot leg at 593OC; wei ht loss 40.9 mg/cm2. Right? in cold leg at 500OC; weight gain 16.0 mg/cm Top: optical micrographs at 500x, etched with glyceria regia Bottom: scanning electron micrographs at 1OOOX.
In loop NCL-20, c
ructed of standar
stelloy N with removable
specimens in each leg, the fluoroborate coolant salt has circulated for 12,000 hr. The salt used was especially pure (see Table 6). The loop is being operated at temperature conditions very near those proposed for the maximum (687°C) and minimum (387°C) salt-metal temperature (primary heat exchanger and steam generator, respectively) of the MSBR secondary circuit. Forced air cooling (as opposed to ambient air cooling used on other thermal-convection loops) is used on the lower half of the cold leg, and the practical operating temperatures obtained were 687°C maximum and about 437°C minimum: a temperature di'fference of 250°C. This difference is thought to be the largest obtained at ORNL in a molten-salt thermal-convection loop, and the maximum temperature is the highest for fluoroborate salt in a loop. Table 6 gives the corrosion results for this experiment. The corrosion rates are the lowest yet attained with a fluoroborate mixture and confirm the importance of salt purity on compatibility with structural materials. The low concentrations of chromium and oxide in the salt are also indicative of low corrosion rates. Figure 14 shows weight changes of the specimens as functions of time and temperature. Table 6. Weight Change of Specimen at 687°C and Impurity Content of Salt of NCL-20
0 624 1460 2586 3784
Weight Loss (mg/cm2>
Incremental Corrosion Rage (mils/year)
0.3 0.7 1.0 1,7 aAssuming uniform loss.
0.19 0.18 0.15 0.17
Chemical Analysis, pym Cr Fe 0
58 90 99
227 198 110
500 550 590 470 670
28 ORNL-DWG 71-8059
<E 5 v
=a o I
685째C HOTTEST SPECIMENS
10,000 12,000 14,000 16,000
TIME OF OPERATION (hr) Fig. 14. Weight Changes of Removable Standard Hastelloy N Specimens in Flowing Sodium Fluoroborate (NCL-20). FCL-1 Pump Loop The MSR-FCL-1 forced-circulation loop operated for over 11,000 hr (7 runs) to test the compatibility of standard Hastelloy N with NaBF4-8 mole % NaF coolant salt at temperatures and flow rates similar ,to those that existed in the MSRE coolant circuit. Salt velocity in the 1/2-in.-OD X 0.042-in.-wall Hastelloy N loop was nominally 10 fps and was limited by the use of an available pump.
The salt in the loop was heated by electri-
cal resistance and cooled by a finned, air-cooled heat exchanger. A schematic of the loop is given in Fig. 15. Figure 16 is a typical temperature profile of the system; this profile was based on a computer plot of the temperature information from the test loop and on heat transfer calculations that estimate the inner wall temperatures. The maximum and minimum salt temperatures of the loop are 588 and 510OC. Hastelloy N corrosion test specimens were exposed to the circulating salt at three temperatures, 510, 555, and 588OC. A typical set of specimens is shown schematically in Fig. 17. One of the main drawbacks to this loop was that the salt had to be drained from the loop and the loop tubing had to
SALT SAMPLE LINE
OIL LINES TO PUMP
I II7 I
HEATER LUG (TYPICAL)
FREEZE VALVE )o- AIR
REYNOLD’S NUMBER -3400 VELOCITY - I fl/sec FLOW RATE - 3 a m
Schematic of MSR-FCL-1. ORNL-DWG 69-2535
WMP LlOUlD TEMPERATURE
Fig. 16. Temperature Profile of Molten-Salt Forced-Convection Corrosion Loop, MSR-FCL-1, at Typical Operating Conditions.
Specimen in Molten Salt Corrosion Forced-Convection
Loop. be cut to remove the specimens. This, of course, necessitated welding to replace the specimens and resulted in a fairly long turnaround time between runs. After 659 hr of shakedown operation under various conditions and the initial 2082 hr of operation at design conditions a bearing failed in the LFB centrifugal pump. The pump rotary element was removed, and a new bearing was installed. To take advantage of this unscheduled downtime, portions of the loop piping and the corrosion specimens were removed for metallographic examination and weight change measurements. This first operating period was designated run 1. It was then decided that the loop would be shut down each 2000 hr for pump-bearing replacement and specimen examination. The operating times and corrosion rates for the first five runs are summarized in Table 7, and Fig. 18 shows the weight changes of specimens as measured after each run. The details of each run will be discussed in the following pages. It is noted that the mass transfer rates were higher in the pump loop than in thermal-convection loops circulating salt of equal purity.
Thus, a velocity effect is suspected.
31 Table 7.
Average Weight Change of Specimens in MSR-FCL-1
Total Salt Exposure Time, hr Run
Average Specimen Weight Change at Indicated Temperature, mg/cm2
Design Isothermal Conditions Conditions 51OOC
Corrosion Rate at 588OC Assuming Uniform LOSS,^ mils/year Overall
a Based on total salt exposure time.
6Ooo 8000 'SALT EXPOSURE TIME (hr)
Fig. 18. Weight Changes of Removable Standard Hastelloy N Specimens in Flowing Sodium Fluoroborate in Pumped Loop MSR-FCL-1. A 1-mil/year corrosion rate is included for comparison. i
32 Runs 1 and 2 Figure 19 shows micrographs of specimens from each location after 2082 and 4088 hr (run 2) of design operation. In (a) and (b) it is clear r
that the attack at 588"C, the highest salt temperature, occurred primarily at the intersections of the grain boundaries with the surface. At 555"C, as the weight changes indicated, much less attack has occurred [(c) and For 510째C, the lowest salt temperature, a metallic deposit is (d)]. visible [(e) and (f)] along the surface in the as-polished condition. This deposit occurs under steady-state conditions and was shown by electron microprobe analysis to have the approximate composition of Hastelloy N; no salt-like deposit was observed. Figure 20 shows the surface of the specimens at 588 and 510째C. Note the smoothness of the surface of the specimen that has been attacked and the deposit on the specimen in the cold region. Samples of loop tubing were periodically removed and examined metallographically for comparison with the weight-change specimens. The behavior was similar, as shown in Fig. 21. The attack concentrated at the intersections of the grain boundaries with the surface, and deposits were seen in the cold region. The tubing had a much smaller grain size than the specimens; from this one might anticipate a greater corrosion rate for the tubing. No difference could be seen between tubing exposed under the heaters and tubing at the same temperature but not under the heaters. Examination of the pump (Fig. 22) and the pump bowl (Fig. 23) did not disclose any gross contamination; however, small amounts of a green material were found on the pump bowl at the salt level. After the bowl was washed with water to remove the salt, very fine, whisker-like, green crystals were also found in the bottom of the pump bowl (Fig. 24). A large piece of mixed green material and white salt (< 1 g total weight) was analyzed and identified; Table 8 shows the composition. These results are equivalent to 55 wt % NaBF4, 30 wt % Na,CrF6, and smaller amounts of iron, nickel, and molybdenum fluorides. The presence of the green corrosion product and the level of chromium concentration in the salt indicate that we reached the saturation concentration of chromium
Fig. 19. Standard Hastelloy N Specimens from MSR-FCL-1, Exposed to NaBFb-8 mole.% NaF for the Indicated Times and Temperatures and for an Additional 659 t o 667 hr at Varyihg Conditions. (a) 588"C, 2082 hr, weight loss .12.5 mg/cm2, etched with glyceria regia, 500X. (b) 588"â‚Ź, 4088 hr, weight loss 18 mg/cm2. (c) 555"C, 2082 hr, weight loss 3.0 mg/cm2. (d) 555"C, 4088 hr, weight l o s s 4 mg/cm2. (e) 510"C, 2082 hr, weight 'fain 2.2 mg/cm2, as polished. (f) 510"C, 4088 hr, weight gain 4 mg/cm
Fig. 20. Surface of Standard Hastelloy Specimens Exposed i n Loop MSR-FCL-1 f o r 2082 h r a t Design - Conditions (and 659 h r a t Varying Condit i o n s ) . 45x. (a) Smooth s u r f a c e on specimen t h a t l o s t 12.5 mg/cm2 a t 588OC. (b) Deposit on specimen t h a t gained 2.2 mg/cm2 a t 510OC.
Fig. 21. Standard Hastelloy N Loop Tubing from MSR-FCL-1 Exposed t o NaBF4-8 mole 4 NaF f o r 2082 h r a t Design Conditions. 500X. (a) Tubing exposed a t 588OC. Etched with g l y c e r i a r e g i a . (b) Tubing exposed a t 510OC. As polished.
Fig. 22. Pump Impeller from Loop MSR-FCL-1. This impeller operated in NaBF4-8 mole % NaF for 659 hr under variable conditions and 4088 hr of normal operation at 510OC.
Fig. 23. Pump Bowl from Loop MSR-FCL-1. The pump operated in NaBF44 mole X NaF for 659 hr under variable conditions and 4088 hr of normal operation at 510OC.
Fig. 24. Inside of Pump Bowl from Loop MSR-FCL-1 After Being Washed with Water to Remove Salt, Showing Crystalline Residue. The pump operated in NaBF4-8 mole % NaF for 659 hr under variable conditions and 4088 hr of normal operation at 510OC. Table 8. Chemical Composition of Green Deposit Removed from the Pump Bowl After Run 2 Element Cr Fe Ni Mo Na
Concentration, wt %
6.14 0.26 0.30 0.022 21.6 4.56 57.0
37 corrosion product in the pump bowl during the test. No indication of 8
fluoride deposit or plugging in any other part of the system has been <;., y.< -. seen. '3
Run 3 Figure 25 shows micrographs of specimens in MSR-FCL-1 after more than 6000 hr salt exposure (3 runs). Uniform attack is seen on the specimens exposed to salt at 588 and 555"C, with the rougher surface seen on the higher temperature sample. In ( c ) the mounting material remclved some of the deposit on the cold-leg specimen, but portions can still be seen. Visual examination of the pump and pump bowl after run 3 showed no obvious corrosion. None of the green Na3CrF6 corrosion product that had been observed previously was present.
Fig. 25. Standard Hastelloy N Specimens from MSR-FCL-1, Exposed to NaBF4-8 mole % NaF for 667 hr under Variable Conditions and 6097 hr at Design Conditions. As polished, 500~. (a) Exposed at 588"C, weight loss 21.4 mg/cm2. (b) Exposed at 555"C, weight loss 4.7 mg/cm2. (c) Exposed at 51OoC, weight gain 5.0 mg/cm2. The light material away from the surface of the sample is part of the surface deposit that became separated from the sample during mounting.
Installation and Testing of Cold Finger During Run 3 During run 3 a cold-finger corrosion product trap, shown in Fig. 26 and similar in design to one previously used25 in sodium fluoroborate test loop PKP-1, was inserted into the salt in the pump bowl in an attempt to induce preferential deposition of corrosion products from the salt circulating in the loop. Such deposition had been observed on the cold finger in loop PKP-1. Gross deposition is always possible in a temperaturegradient system, and we feel that this cold-finger device is a likely component to prevent this problem. The cold finger used in MSR-FCL-1 is a closed-end nickel cylinder, 1 3 / 4 in. long X 3/8 in. OD, with a 0.070-in.-thick wall. It is cooled by an argon-water mixture injected into it and then discharged to the atmosphere. The metal wall temperature is measured and recorded by two O.OZO-in.-OD sheathed, ungrounded Chrome1 vs Alumel thermocouples inserted in two 1-in.-deep axial holes (0.023 in. diam) in the 0.070-in.-thick wall of the â€™ cold finger. 25A. N. Smith, P. G . Smith, and R. B. Gallaher, MSR Program Semiann. Progr. R e p t . Feb. 28, 1969, ORNL-4396, p. 102.
Fig. 26. Cold-Finger Corrosion Product Trap for MSR-FCL-1.
39 ’Eight tests were made in which the cold finger was inserted into the salt in the pump bowl of the loop and cooled to temperatures ranging from 493 to 14OoC, The duration of the tests ranged from 1.5 to 5.3 hr. The temperature of the salt in the pump bowl was 510°C. In contrast to the deposits of material containing NajCrF6, which had been found26 on a cold finger in PKP-1 loop at metal wall temperatures of 400, 460, and 477”C, no significant deposit of any kind was seen on the cold-finger tests in loop MSR-FCL-1. Even in the three tests where indicated wall temperatures were below the salt liquidus temperature (385OC), the surface of the cold finger was essentially clean, as visually observed when it was withdrawn into a sight glass. Occasionally, small patches (l/8 to 1/4 in. across) of white material, estimated to be a few‘milsthick, were seen on the surface. The cold finger was then installed in the PKP-L fluotoborate loop -n an attempt to duplicate the previous cold-finger test results of that loop.
The chromium concentration of the fluoroborate salt in loop PKP-1 is about 500 ppm, while that in MSR-FCL-1 is about 250 ppm. Two ‘tests were run in which the indicated cold-finger wall temperature was about 15OOC (salt temperature in the pump bowl was 548OC).
were 1 and 4.5 hr. No deposition on the cold finger was seen after withdrawal into a sight glass.
Tests at higher temperatures were not
made because of .temperature control difficulties with the cold finger. Since the cold finger previously used in the PKP-1 loop coatained grooves on the outside surface, the lower half of the surface of the MSR-FCL-1 cold finger was scored with file marks about 0.010 in. deep, and a third test run at about 15OOC lasting 6 1/2 hr was made in the PKP-1 loop. In this run a’deposit was obtained. Generally, the entire ’surfaceof the cold finger was covered with a white deposit, with an overlay of bright green material on the lower half of the cold finger. The cold finger was allowed to stand overnight under a helium atmosphere, II ’
and by this time the deposit,had begun to separate from the cold-finger surface. While the cold finger was moved for photographing, the entire
’ 26R. B. Gallaher and A. N. Smith, MSR Program Semiann. Progr. . R e p t . Aug. 31, 1969, ORNL-4449, pp. 74-75.
deposit spalled off, leaving a clean metal surface. The total deposit weight was 1.63 g, of which 1.26 g was mostly green material (complete separation was not possible). Chemical analysis of the green material disclosed 2.93 wt % Cr, 1.03 wt X Fe, 370 ppm Ni, and < 500 ppm Mo, with the remainder Na, B, and F. Stoichiometric calculations indicated I 11 mole % Na3CrF6, 4 mole % NasFeF6, and the remainder a mixture of NaBF4 and NaF. Subsequent operation of the cold finger at the same conditions in loop MSR-FCL-1 did not produce a deposit. On the basis of these tests we concluded that a wetting problem exists with the salt and that a grooved or roughened surface is required to obtain a deposit. We then tried various designs to improve adherence of the deposit to thescold finger and to lessen the probability of accidental removal during withdrawal from the pump bowl. Run 4 After,run 4 when the pump had been removed, we found approximately 50 g of intermixed white and green material on the pump liner above the liquid level. Analysis of a small portion of this material showed about equal amounts of NaF and NaBF4, with 4300 ppm Cr, which we assume to be in the form of NasCrF6. We do not know the conditions that caused the deposition of the corrosion product in the pump liner. Specimens in the coldest part of the system gained weight during the first three runs and then lost a small amount of weight during run 4. Thickness measurements of these specimens disclosed that the upstream end had reduced in thickness compared with the middle and downstream end.
Specimens at other locations in the loop (555 or 588OC) showed
similar but smaller thickness variations.
Figure 27 shows a specimen
at 588째C after run 4 and clearly illustrates the heavier attack at the upstream end. Changes in specimen thickness are summarized in Table 9,
and they are quite consistent with the changes calculated from weight measurements. Figure 28 shows micrographs of specimens from MSR-FCL-1 after run 4
(9600 hr total exposure to the fluoroborate mixture). The left micrograph shows the surface of the specimen at the hottest position (588OC).
41 PHOTO 77729
Fig. 27. Hastelloy N Specimen 4 from MSR-FCL-1 Exposed to NaBF4-8 mole X NaF at 588째C for 9600 hr (Through Run 4). Flow is to the left. Table 9. Average Thickness Change of Specimens After 9600 hr Total Exposure to NaBF44 mole % NaF in MSR-FCL-1 Specimen Temperature
Average Thickness Change (mils)
a Discounting upstream end of sample, thickness increase is +2.5 (see text).
Temperature, *C Weight Chage, me/.n?
Fig. 28. Hastelloy N Specimens from MSR-FCL-1 Exposed to NaBF4-8 mole % NaF for 9600 hr (4 Runs).
Average weight losses of the specimens are 21.3 mg/cm2. Microprobe analysis disclosed a concentration gradient of chromium and iron for a distance of 0.6 mil. There is less than 1.0 wt % Cr and only 1.0 wt % Fe 0.4 mil into the specimen. This depleted area is represented by,the darkened area extending from the surface for approximately 0.5 mil. The center micrograph shows the surface of a specimen at 555째C. The average weight loss of these ,specimens was 4.6 mg/cm2. Microprobe analysis of these specimens disclosed only a small concentration gradient for a distance of 0.1 mil. This follows from the small amount of attack seen on the specimen. The micrograph to the right shows the deposit on the surface of the specimens at 51OOC. The average weight loss of the specimen is 0.1 mg/cm2, but this overall loss stems from a great deal of corrosion on the leading edge and is not indicative of the whole specimen. Microprobe analysis of this surface showed a large amount of iron and a little more nickel than usual.
This situation existed for a distance of 0.5 mil,
after which the concentrations of both elements approached that of the matrix. The average deposit is only 0.2 mil thick; thus, it appears that portions of the deposit have diffused in. Prior evidence in deposit study had disclosed similar findings. Run 5 Run 5 was terminated after 422 hr of operation at design conditions when the pump bearings failed. This failure allowed the pump impeller to contact the impeller housing, abrading the impeller. Metal particles from the impeller were seen in the salt left in the pump bowl after dumping. Accordingly, the pump was removed from the loop, and at the same time we removed the corrosion test specimen assemblies. This allowed us to clean the loop piping by flushing with demineralized water. A total of 3.31 g of Hastelloy N particles was recovered from the loop.
The loop was dried by air purging, and the corrosion specimen assemblies and pump were reinstalled. A nickel filter with 40-pm pores was also installed in the dump tank line to filter any metal particles from the salt being returned to the loop. During the scheduled loop shutdown at the end of run 4, we had enlarged the access port in the pump bowl from 112- to 3/4-in. diam
(maximum size possible in the pump bowl) to provide more flexibility in the design and operation of cold-finger devices. With the enlarged access port we were able to insert a 5/8-in.-OD cold finger with circumferential grooves that had been previously used in another circulating fluoroborate loop (PKP-1) and on which significant deposits of salt containing NasCrF6 had been obtained. Several tests were made during run 5 with this cold finger at temperatures between 150 and 420OC. The cold finger was inserted below the liquid surface in the pump bowl for periods of 5 to 6 hr for each test. The salt temperature in the pump bowl was approximately 516OC. Small deposits with a light-green color (indication of corrosion product Na3CrF6) were occasionally seen on the cold finger when it was withdrawn into the sight glass above the pump bowl. However, such deposits usually dropped off immediately. Apparently any slight vibration is enough to knock most of the deposited material loose before the cold finger can be .pulled all the way out of the pump bowl. The weight changes of Hastelloy N specimens in loop MSR-FCL-1 are
compared in Table 7 for each of five test runs. The corrosion rate decreased steadily over the first four runs and, at the conclusion of run 4, had dropped to 0.3 mil/hr at the point of maximum temperature However, the corrosion rate during run 5 was higher than in (588OC). any of the preceding runs. Although the increased rate of attack during run 5 is undoubtedly associated with operating difficulties encountered during the run, we have not pinpointed the specific causes. Increased corrosion is normally accompanied by an increase in impurities in the salt; however, we did not see any significant impurity changes during run 5. Because of the nature of the last pump-bearing failure, we were not able to take a salt sample from the loop before shutdown in our normal manner. Thus a sample
was taken from the dump tank after the loop had been shut down. However, because of dilution there was no assurance that the sample was representative of the salt that had circulated in the loop. Figure 29 shows specimens 2 (555OC), 4 (588OC), and 8 (510OC) at the end of run 5. Note the change in appearance 'of specimen 4 between run 4 (Fig. 27) and run 5 (Fig. 29). The etched appearance of specimen 4 after
. . ..
. . .. ..
Fig. 29. Hastelloy N Specimens from MSR-FCL-1 Exposed to NaBF4-8 mole % NaF for 10,000 hr Total (Through Run 5). From top to bottom the temperatures were 555, 588, and 510OC.
run 5 is typical of the appearance of Hastelloy N specimens in thermal convection loop NCL-17 (see previous section,,%Fig. 13) after extreme oxidizing conditions had been created by intentional steam inleakage and large amounts of mass transfer had occurred. Run 6
The sixth run was abruptly terminated after 1241 hr, when oil from a broken pump cooling oil line ignited on contact with the pump bowl and adjacent piping. We extinguished the fire and turned off all loop heaters, which allowed the salt to freeze in the loop piping. Figure 30 shows the pump bowl and pump with no apparent damage after the fire. The material in the beaker is salt and corrosion products left in the pump bowl. We replaced the electrical wiring, thermocouples, and service piping necessary to melt the salt in the loop piping and transfer it to the drain tank. This was the first time that we had attempted to melt c
salt in the entire loop circuit, although salt had been melted in the cooling coil without difficulty on several occasions. Normally when the loop is placed in standby condition, the salt circulation is stopped,
Fig. 30. Standard Hastelloy N Pump from MSR-FCL-1. Impeller exposed to NaBF4-8 mole X NaF 1319 hr; baffles exposed 11,371 hr. Outside of the pump was exposed to oil fire.
46 the main loop heaters are turned off, and sufficient heat is supplied to the loop to maintain the loop circuit above the salt liquidus tem,perature,385OC. During the attempted melting, the main loop piping (1/2-in.-OD X 0.042-in.-wall Hastelloy N) ruptured at a point near the U-bend in the loop and adjacent to one of the metallurgical specimen holders, as shown in Fig. 31. After the rupture, we froze the salt in the loop as quickly as possible by turning off all loop heaters. However, approximately 77 g salt was lost from the loop. Before the rupture the salt in the bowl and cooling coil section of the main loop had been melted without difficulty, the main loop piping had reached temperatures varying between 371 and 482째C around the loop circuit, and the drain line temperatures were above 426OC.
Fig. 31. Molten-Salt Corrosion Testing Loop MSR-FCL-1 and Power Supplies Showing Points of Rupture in Runs 6 and 7.
In reviewing the loop melting procedure to determine the cause of the rupture, we concluded that uneven thicknesses of thermal insulation caused considerable variation in the temperatures.
In particular, the
temperatures under the clamshell emergency heaters (where the thermal insulation was about 1 in. thick, compared to about 2 in. on the remainder of the tubing) were about 80째C below temperatures in the more heavily insulated sections of tubing. Thus, the salt in the ruptured area melted . but was not able to expand properly because of frozen salt plugs under the emergency heaters. Another problem was the difficulty in controlling the rate of heatup of the main loop by resistance heating. Even though
the lowest setting on the loop heater was used, we still had to turn off the heater supply power for short periods to maintain temperature control. We removed the metallurgical specimen assembly and ruptured section of tube and replaced it with new tubing. Figure 32 shows the ruptured section of tubing. Measurements of the outside diameter of the remaining loop tubing were made and compared with the original outside diameter to determine if excessive permanent strain had occurred at other locations.
Fig. 32. Tube Ruptured During Salt Melting after Run 6 , Loop
48 Generally all measurements were in the range of 0.500 to 0.505 in., as compared to the original diameter of 0.500 in. The tubing that surrounded the specimens was removed after run 6
(11,371 hr) and examined by both optical metallography and scanning electron microscopy. Figure 33 shows the tubing exposed to salt at 588 and 555OC. In the optical micrograph of Fig. 33(a) the surface roughening (some salt is still in place) can be seen, and the attack at the grain boundaries is noted. In the scanning electron micrograph we can see the delineation of the grains. Figure 33(b) shows much less attack at 555OC. Figure 34 shows the tubing downstream of the cooler in the coldest position (51OOC) of the loop. The deposit is easily seen in the optical micrograph and is seen in the scanning micrograph to be in the form of nodules. The upper portion of Fig. 34(c) shows a side view of the nodular deposits. After the oil fire that ended run 6 and the subsequent rupture of the tubing during the attempt to melt the salt from the loop, the corrosion specimens were removed, weighed, and examined. Surprisingly, weight was lost by all specimens. The weight loss rates found for specimens exposed to the salt at 588 and 555째C were (assuming uniform losses) about 1.9 and 0.5 mils/year, respectively, for the 1240 hr of run 6 . The corrosion rate ratio for these spec'imens (several times greater loss at 588OC than at 555OC) was fairly consistent with past findings. However, in earlier runs, specimens at 51OOC had gained weight. For this time period specimens at this temperature level lost material at the rate of 1.9 mils/year, the same as for specimens at 588OC. This weight loss anomaly and the overall higher weight losses are attributed to the problems encountered during this run and probably attest to a local high temperature in the colder section along with oxidizing impurities in the salt. A salt analysis showed small increases in chromium, iron, and nickel contents, all of which reflect the increased corrosion rates.
Run 7 After repairs we returned the loop to design conditions for the start of run 7, circulating the same NaBF4-8 mole X NaF coolant salt used since the start of loop operation.
Fig. 33. Hastelloy N Tubing from MSR-FCL-1 Exposed to NaBF4-8 mole X NaF for 11,371 hr. Left: optical micrographs, SOOX. Right: scanning electron micrographs, 1OOOX. Top: at 588째C and bottom at 555째C during design operation.
Fig. 3 4 . Hastelloy N Tubing from MSR-FCL-1 Exposed to NaBF4-8 mole % NaF at 51OoC for 11,371 hr. (a) Optical micrograph, 500X. (b) Scanning electron micrograph, 1 0 0 0 ~ . (c) Scanning electron micrograph, 3000X, taken with the specimen tilted to give a side view.
During run 7 while repairs were-underway on the loop high-temperature 'protectiveinstrumentation, an operating error resulted in a portion of the loop tubing bein ted above 1100째C. is caused one failure of the loop tubing adjacent to one of the electrical power input lugs (see Fig. 31) and also about 12 in. downstream. Part of the salt in the loop (about 2 liters) was discharged into the loop secondary containment. Temperatures were immediately reduced and the facility was shut down. At about 1100째C the strength of Hastelloy N is very low, and the salt vapor pressure approaches 1000 psi. The salt boiled locally, and overheating could have reduced the tube strength until rupture occurred. Local melting of the tubing was also evidenced. At the time of failure the loop had accumulated 10,335 hr of operation at design conditions (101 hr during run 7).
The tube failure is shown in Fig. 35.
Following the rupture of the loop tubing that ended run 7, the corrosion test specimens were again removed for weighing and metallurgical examination. The specimens adjacent to the ruptured area (hottest section under normal conditions, 588째C) were badly warped and partially fused to the tube wall. Thus, only metallographic analysis was possible. The specimens in the intermediate zone (555OC) appeared to be unharmed. The average weight loss for these specimens was 1.3 mg/cm2 in the 101 hr of run 7.
Expected loss for these specimens in 100 hr would be approximately 0.1 mg/cm2. Thus, if we attribute the balance of the corrosion to just the period of the temperature excursion (to about lOOO"C), the loss rate was 1.2 mg/cm2 in 2.5 min or 10,000 mils/year (10 in./year). Weight losses were also found for the specimens downstream of the cooler. Although the specimens were adjacent, one specimen lost 0.3 mg/cm2 and the other 3.0 mg/cm2. Again the severity of the overheating wae evident. Certainly a large part of these losses may be' I attributed to moisture contamination of the salt and air oxidation after the loop rupture. Nonetheless, the corrosion rate was quite high. The loop is now being modernized and prepared for additional service.
53 SALT CHEMISTRY Purification With the realization that the fluoroborate salt is easily contaminated with oxygen and water-type impurities and that corrosion increases with the amount of these impurities, we have attempted, in close cooperation with R. F. Apple and A. S. Meyer, of the Analytical Chemistry .Division, to purify the fluoroborate in a manner that could be adapted to a large system. In the method that gave favorable results, a'mixture of He, BF3, and HF (purified with fluorine) was passed through the fluoroborate at 454째C. 'A schematic of the process is given in Fig. 36. The gas mixture was passed for 15 hr into a Hastelloy N vessel containing the impure (about 2000 ppm H20) fluoroborate salt (2.7 kg) at 48OOC. The exit gas entered a solution of 10 vol X pyridine in methyl alcohol. At the completion of the purification process titration of this solution with Karl Fischer .reagent to the dead-stop end point indicated that about 600 'ppm d H 2 0 was removed. Chemical analysis disclosed that the oxygen content 'decreased from 1700 to 1400 ppm and that the H20 content changed
ORNL-DWG 69- 12547R
END POINT INDICATOR
NoBF4- NoF(92-8 mole %I 450 SOo C ORIGINAL 2000 ppm H P
o METHYL ALCOHOL PYRIDINE
AFTER i 5 hr SPARGING 3OD pprn H P
System for Removing Water from Coolant Salt.
54 from 2000 to 300 ppm.
Changes in the BF3 content of the salt appeared
to be minimal.
Further work is planned using a nickel vessel to eliminate corrosion products resulting from the reaction of HF with Hastelloy N.
Analytical Chemistry Over the last few years, we have been concerned over the be.havior of water in molten fluoride salts. Water in these salts has implications for both corrosion and tritium removal. In corrosion work, we have long recognized the need for analyses that would allow us to distinguish
between water and (1) compounds that contain H ions, (2) compounds ' ions, and (3) HF (highly corrosive). In the past, a which contain 0 complementary indication of mass transfer (besides weight changes and
metal analysis of the salt) was the analysis for H20 and
in the salt.
On the basis of our tritium injection experiment27 and work in the
Analytical Chemistry and Reactor Chemistry Divisions, we now feel that the results of the water determinations included many other constituents of the salts, including oxides. Thus, a result indicating a large amount of water really only showed a corresponding amount of oxide. The lack of water in in impurity tion of the which would
the salt is completely reasonable because all the hydrogen compounds that enter the salt would eventually cause oxidametal wall and would in turn be reduced to hydrogen gas, diffuse out of the loop (the corrosion equations will be
discussed later). However, increased mass transfer (weight losses and gains by specimens) by virtue of water impurity is still accompanied by an increase in the oxide content of the salt. Thus, the oxide content is still somewhat indicative of the mass transfer of the loop system.
DISCUSSION Theory t
Metal corrosion by salt mixtures consists of oxidation of metal constituents to their fluorides, which are soluble in the melt and hence 2 7 5 . W. Koger, MSR Program Semiann. Progr. R e p t . Feb. 28, 1971, ORNL-4676, pp. 210-11.
do not form a protective film. This electrochemical-type attack is therefore limited only by the thermodynamic potential for the oxidation reaction and is selective, removing the least noble constituent, which in the case of Hastelloy N is chromium. Possible corrosion reactions involving impurities in the melt may be written as 2HF
+ Cr + Cr
Although the reaction product is written as CrF2, the actual species in the melt is unknown. Chromium(I1) is possibly unstable in the fluoroborate melt, since the only corrosion product isolated and identified is NasCrF6. Table 10 illustrates the thermodynamic stability of the fluoride compounds in question. Table 10. Relative Thermodynamic Stabilities of Fluoride Compounds
Most Stable Fluoride Compound
Standard Free Energy of Formation (kcal/g-atom F) at 8OOOC
Fe Ni Mo
FeF2 NiF2 MOF 5
-66 -59 -57.
-69 -63 -58
Na K Be
-110 -108 -103
-113 -100 -96
In an isothermal system, immediately after immersion in the fused salt system and before thermodynamic equilibrium has been fully established, the electrode potential of the metal has a much higher electronegative value than the redox potential of the surrounding medium. As
a result, reduction of the oxidizer commences which takes place along
As the corrosion products accumulate the metal's electrode potential shifts in the positive direction, whereas the redox potential moves toward the negative side. Equilibrium occurs when the potentials are equal. Since we are dealing with corrosion in a nonisothermal system (i.e., a heat exchanger), the mechanism of interest t o us is temperature-gradient mass transfer. A schematic of this process is given in Fig. 37. In a loop that contains salt with UFI, and no corrosion products, all points of the loop initially experience a loss of chromium by the reaction with the corrosion of the metal.
+ Cr SCrF2 + 2UF3.
As the corrosion-product concentration in the salt is increased, equilibrium with respect to the corrosion reaction is eventually reached at the point of lowest temperature of the system. At regions of higher temperature, a driving force for the corrosion reaction still exists. Thus, the corrosion-product concentration will continue to increase and the equilibrium temperature will beg& to increase from the coldest temperature. At this stage, chromium is returned to the walls of the coldest point of the system. The rise in corrosion-product concentration in the circulating salt continues until the amount of chromium returning to the walls exactly balances the amount of chromium entering the system in the hot-leg regions in the same interval. Under these conditions, the two positions of the loop at equilibrium with the salt, which are termed the "balance points," do not shift measurably with time. Thus, a quasi-steady-state situation is eventually achieved, whereby chromium is transported at very low rates and under conditions of a fixed chromium surface concentration at any given loop position. At this point the chromium removal i s controlled by the solid-state diffusion rate of chromium in Hastelloy N. Table 11 illustrates the small
HOT SECTION DIFFUSION TO SURFACE
SOLUTE ESCAPE THROUGH - NEAR-SURFACE LIQUID LAYER DIFFUSION INTO s U E LIQUID
TRANSPORT TO COLD PORTION OF SYSTEM ;
.- - --_ X SUPERSATURATION - -- NUCLEATION o GROWTH TO STABLE CRYSTAL SIZE - ~ _ _ - - ---OR L-
COLD SECTION '
SUPERSATURATION AND DlFFUSlON - THROUGH LIQUiD - - _ _ - NUCLEATION AND GROWTH ON METALLIC WALL - -- OR DIFFUSION INTO WALL - - - a
- F i g . 37.
- - - -
Temperature-Gradient Mass Transfer.
Table 11. Chromium Transfer from Hastelloy N with Surface Concentration Reduced to Zero Diffusion Coefficienta Temperature
Depth of Chromium Gradientb
2 x 10-l~
2 x 10-12
4,000 1.5 16,000 3 . 256,000 (30 years) 12 4,000 12 16,000 18 256,000 (30 years) 70
0.6 1.2 4.7 4.7 7.1 27
a By surface activity measurements and microprobe traces after 250and 500-hr exposures. bChromium concentration within,95% of initial concentration in Hastelloy N (about 7 wt %). amount of chromium that will be removed if oxidizing conditions are minimal and solid-state diffusion is controlling. There should be very little corrosion of Hastelloy N by pure molten NaBF4 or NaF, such as is seen for LiF or BeF2; thus we attribute the mass transfer to other sources. We have shown several examples of inadvertent air (moisture) inleakage and the concomitant increase in mass transfer. This was also illustrated in NCL-17, where steam was added.
The corrosion reactions in the sodium fluoroborate salt mixture
have not been well established but can be expected to be reasonably represented by the following equations:
H20 + NaBF4e NaBF30H + HF, NaBF30H+NaBOF2 + HF,
6HF + 2Cr + 6 N a F s 2NascI-F~+ 3H2 (and similar reactions with nickel and iron), 302 + 4 C r t Xr2O3, Cr2O3 + 3NaBF4 + 6NaFsPNa3CrF6
FeF2 + Cr* CrF2 + Fe (and similar reactions with nickel and molybdenum fluorides).
The ‘next‘result is that water reacts with sodium fluoroborate to
produce hydrogen fluoride and oxide ions or an oxygen-containing complex in the salt. The hydrogen fluoride reacts with the constituents of lloy N to bring metal ions into solution in the salt and to release hydrogen. It is not known if the oxide in solution can corrode Hastelloy N, but oxygen in air can react with Hastell N to produce metal oxides. form metal ions and oxide ions These metal oxides dissolve in the melt in solution. Metal ions in solution in the salt react with and displace . -a
less noble constituents of the HastelJoy N.
Highly oxidizing conditions ce of HF) can bring all the constituents into,solution. AS the
comes less oxidizing the more nsble metals in solution react with less noble alloy constituents until only chromium ions are present in
the salt in important .quantities. This movement of chromium is governed primarily by the rat f diffusion of chromium in the’Hastelloy N. Assuming that H2D (or HF) causes the mass transfer in sodium fluoroborate and on the basis that 1 mole of H20 is required to corrode 1 mole of metal we have calculated the amount of water required to cause known amounts of corrosion on several of our systems (Table 12).
in the 1054-hr operation before steam addition, 41mg H20 would been required to cause,,the137 mg metal removed, leaving 75 ppm in the salt. At the end of 10,000 hr after steam addition 23 g had been removed. This would have required 6.3 g H20 and would
have oxide of metal have
resulted in 13,800 ppm oxide in the salt. Since we have never measured this much oxide in the salt, this material. must deposit. The amount ter required to produce the corrosion seen in NCL-20 is small but ontinued to increase with rime. This can mean several things. One, there.is a constant inleakage in our test systems or, two, there are ent in the salt, which continually cause corrosion. The y is quite plausible because we have seen faulty .gas regulators, which can leak undetected for quite a long time. As for the second possibility, the Fen+ concentration in th alt‘has decreased over
120 ppm, which would result in the removal of only 350 mg of chromium from the Hastelloy N.
This still leaves about 600 mg that we might
attribute to water-caused corrosion.
Calculated Amount of Water Necessary to Remove Experimentally Determined Amount of Metal in Different Loop Systems
Total Material Corrosion Rate Removed From At Position of Hot Leg After Highest A Given Time Temperature (milslyear) (mg)
Oxide H20 Required To Remove Total Resulting From Material Reaction (mg) (mg)
NCL-17 1,054a 239 424 663 1,474 2,888 4,756 6,030' 9,006 10,178
137 3,320 4,150 4,700 6,090 7,200 9,960 12,700 14,400 23,000
3,898 6,173 8,501
349 615 923
958 2,225 3,545 5,339 11,680 14,495 16,843
1,380 1,890 2,340 3,030 5,300 7,030 11,500
2,741 4,747 6,756 9,600 10,000 11,472
11,790 17,690 21,620 23,580 35,370 42,250
0.22 19.4 13.6 9.9 5;8 3.5 2.9 2.9 2.2 3.1 NCL-20 0.17 0.19 0.20 NCL-13A 1.6. 0.95 0.74 0.64 0.51 0.54 0.76 FCL-1 1.7 1.5 1.3 0.96 1.4 1.4
41 996 1,245 1,410 1,827 2,160, 2,988 3,810 4,320
200 5,000 6,000 7,000 9,000 12,800 15,000 19,000 21,600
105 185 277
525 925 1,400
414 567 672 909 1,590 2,109 3,450
2,070 2,850 3,360 4,550 , 8,000 10,550 17,250
3,540 5,310 6,486 7,074 10,611 12,675
17,700 26,500 32,000 35,000 53,000 63,500
a Before steam addition, all other times of loop NCL-17 after steam addition.
The experimental weight changes-ofspecimens in the hot and cold portions of the polythermal systems are functions of time at a given temperature and are expressed by the equation W = a tb
W = weight change in milligrams per square centimeter of surface . area,
a = constant, t = time in hours, b = kinetic time constant. The actual weight loss per unit time is a function of temperature and is represented by the Arrhenius relation
dW =A dt
where -dW =
weight change in milligrams per square centimeter of surface area per unit' time,
A = constant, R gas constant, T = absolute temperature in Q = activation energy.
From Fick's second law of diffusion, one can develop the'equation I
AM = weight of material transported, AZ = internal peripheral area of loop tubing, Pa
= density of original alloy,
Xa = initial chromium concentration, K = equilibrium constant at the balance point, P = equilibrium constant at the absolute temperature T, D = diffusion coefficient of chromium in alloy, and
t = time.
This equation describes the mass transfer that can occur in a temperaturegradient system. The use of equations of this type is given in a paper by Evans, Koger, and DeVan." Of importance is the fact that at the balance point no material is transported, at temperatures above the balance point material is transported away, and at temperatures below the balance point material is brought in. The equation was originally considered only for diffusion-controlled processes such as the corrosion reaction between chromium and UF4, but we see in our plots of weight change versus position that balance points exkst even when solid-state diffusion is not controlling (Figs. 38, 39, 40, and 41). Thus the same mass transfer theory holds for our impurity-controlled reactions. The material deposited in the cold leg during the normal operation of the loop is metallic, generally nickel and molybdenum. Plugging-
type deposits, usually resulting when the solubility of a metal fluoride in the salt is exceeded, have been found to be mixed or complex fluorides such as NasCrF6, NaFeF3, NaNiF3. This report does not include discussions of condition of saturation of any components. Most of the material retained in the salt is chromium with some iron, both in tbe form of fluorides. Kinetics According to prevailing concepts of reaction mechanisms, a reaction such as the corrosion of a solid material by a fused salt occurs as a sequence of steps. The combined effect of these steps determines the net rate of the reaction. However if, as is common, one step is "R. B. Evans 111, J. W. Koger, and J. H. DeVan, Corrosion in Polythermal Loop Systkms. II. A Solid-state Diffusion Mechanism With and Without Liquid Film Effects, ORNL-4575, Vol. 2, (June 1971).
. - ,
Fig. 38. Weight Change as Function of Position (Temperature) for Titanium-Modified Hastelloy N Exposed to Sodium Fluoroborate Salt in EOOP NCL-14. 4
0" I w I-
424 hr 663 hr 1474 hr 2888 hr 4756hr 6030hr 9006hr 10.178 hr 1054 hr
TIME AFTER STEAM INJECTION
10 20 30 40 50 60 70 80 90 DISTANCE FROM HOTTEST PORTION OF THE UPPER CROSSOVER (1n.1
COLD LEG (VERTICAL 1
++-- Ji--t------ --I BEND LOWER BEND HOT LEG CROSSOVER
IO 20 30 40 50 60 70 80 90 DISTANCE FROM HOTTEST PORTION OF THE UPPER CROSSOVER (in.) I I
COLD LEG (VERTICAL)
BEND LOWER BEND CROSSOVER
HOT LEG (VERTICAL)
Fig. 39. Weight Change as Function of Position Fig. 40. Weight Change as Function of Position (Temperature) for Hastelloy N Exposed to Sodium (Temperature) for Hastelloy N Exposed to Sodium Fluoborate Salt in Loop NCL-13A. Fluoborate Salt in Loop NCL-17.
65 ORNL-WVG 79-8061
IO 2Q 30 40 50 60 70 80 90 DISTANCE FROM HOTTEST PORTION OF THE UPPER CROSSOVER (in.)
__- UPPER CROSSOVER
COLU LEG (VERTICAL)
BEND LOWER BEND CROSSOVER
HOT LEG (VERTICAL)
Fig. 41, Weight Change as Function of Position (Temperature) for Hastelloy N Exposed to Sodium Fluoborate Salt in Loop NCL-20.
significantly slower than the others, the rate of the entire reaction is governed by the slowest step. It is convenient to break up the dissolution process in the hot leg into four separate steps: 1. diffusion of the attacked elements through the matrix of the alloy to the surface, 2, migration of the oxidizing species from the salt to the surface, 3.
oxidation of the metal to a dissolved fluoride, migration af the oxidized metal to the flowing salt. In cases where the slow step involves a diffusion process (volume
diffusion in a solid), the reaction is termed diffusion-controlYed and is governed by the laws of diffusion kinetics, Alternately, if a boundary-region process.(solution) constitutes the slow step, the rate of the overall reaction is determined by the kinetics of that process.
The rate of formation of the corrosion product fluoride should be included
in this analysis, but experimental data relating to its formation and
the effect of impurities are lacking. If the diffusion step is rate controlling, then no velocity effect would be seen. However, if step 2 was slowest and was controlling, the . process would be velocity dependent. At a certain critical velocity (possibly even that of the salt in natural circulation loops), the path for step 2 would become short and step 3 would control. Above this critical velocity, no velocity dependence would again be seen. Step 4, like step 2, would be velocity dependent. Thus, experiments in systems with different salt velocities could help to determine the rate-controlling mechanism. In this work, we will consider the possibilities of solid-state diffusion and solution control. Solid-state Diffusion Control A form of Fick's second law can be used for the weight loss in this case W=AC&, where W
C = concentration change of diffusing substance, D
solid state diffusion coefficient,
t = time,
A = constant. If Eq. (4) applies, b of Eq. (1) is theoretically equal to 1/2. The diffusion coefficient follows the Arrhenius relationship
where Do is constant and Ds is the effective activation energy for diffusion in the alloy.
If we differentiate Eq. (4) and substitute Eq. ( 5 ) for D, we obtain
AC -2 J&F .eXp<-Ds/2RT)
showing that the theoretical activation energy for the corrosion reaction is half that for diffusion: Qtheo = Ds/2 Solution Controlling The following type of equation is used2' to describe solution attack controlled by liquid diffusion in a thermal gradient system ,
dt where V
~ 6,,-0 ~
velocity, kinematic viscosity,
DL = diffusion coefficient in the liquid, d = diameter of pipe, p = density of liquid,
solubility of container material in liquid. The diffusion coefficient can be expressed by the Stokes-Einstein relation S =
k = Boitzmann constant, q,
X = radius of diffusing ion, Q, =
actgvation energy â‚Źor viscosity.
29G. W. Horsely, "Mass Transport and Corrosion of Iron-Based Alloys in Liquid Metals," J . NucZ. Energy P u r t B: Reactor T e c h Z . 1: 84-91 11959).
The kinematic viscosity can be expressed as
and the solubility as S = S o exp(-AH/RT)
where S o is a constant and AH is the heat of solution. From the temperature dependence on dW/dt in Eq. (7) after substitution using Eqs. (8), (9), and (lo), we can obtain for the theoretical heat of activation of corrosion
+ RT(0.6 + 1 . 4 : g ) + AH
Comparing Eq. (11) with experiment2â€™ shows that at least 80% of Qtheo is the value of AH, the heat of solution of the corrosion product in the fluid. Thus we take Qtheo = 1.25 AH For this system btheo
Experimental Data The heats of solution of FeF2 and NiF2 in molten fluoride salt are about 12 and 8 kcal/mole, respectively.3o The average value 10 kcal/mole will be used for AH. A value of 60 kcal/mole will be used for the effective activation energy, D,, for volume self-diffusion for iron and chromium. Table 13 compares the Qtheo and theo for the two proposed corrosion mechanisms with experimental values of Q and b for the specimens in the systems that lost material. Values are given for the coolant salt at two different impurity levels. One might imagine that at the beginning of a mass transfer experiment diffusion of the elements through the matrix would not play a large part 30C. M. Blood, F. F. Blankenship, G. M. Watson, W. R. Grimes, Reactor Chem. Diu. Annual Progr. Rept. Jan. 31, 1960, ORNL-2931, pp. 39-43.
69 Table 13.
Rate Expressions for Materi-1 Removed in Coolant Salt NaBF4-8 mole X NaF Oxide Content TemperaOf Salt ture (PPd ("0 500
Hastelloy N Standard Hastelloy N
3 x io4
1 x io5
555 Ti-modified Hastelloy N
a 0.0036 0.0025
Temp erature Dependenceb
Weight Change Constantsa
Theoretical Values Diffusion control
Solution rate control
aConstants for equation W = atb, where W = weight change, mg/cm2; t = time, hr.
. dW = A exp(-Q/RT) dt bConstants for equation in the process since the material which is to be removed is already at the surface. Thus, step 2, 3, or 4 might be controlling. After the initial fast portion of the reaction the corrosion rate generally levels out.
At this time, the diffusion of the elements to the surface would
Thus, the calculated overall rate would appear to be of mixed control. When a velocity effect is noted, as is thought to occur control.
in MSR-FCL-1, then -it can be assumed that enough impurities are,controlling the corrosion reactions to cause solution rate control of the entire process. Although the proposed corrosion mechanisms are usually first considered for material removal, they may also be used for the deposition in the
cold leg of the system. The temperature dependence is reversed, the largest deposition occurs at the highest temperature, which causes a change in sign of the activation energy. Table 14 gives the experimental values of Q and b for the systems which gained weight. The'kinetic constants of one group, titanium-modified alloy and fluoroborate salt with 1500 ppm oxide, corresponds to solid-state diffusion control, but the value of the others are in mixed agreement.
Diffusion Calculations Weight change rate constants based on diffusion control were calculated for loops NCL-13 and NCL-14 after 2500 hr with the following equation: Awloss = C /-, where C
concentration of Fe
T > 520 & 15OC
in Hastelloy N, g/cm3,
D = diffusion coefficient, cm2/sec, t = time, sec. By using the weight changes and the combined iron and chromium concentration for the loop specimens, almost identical D values were obtained for the standard and modified Hastelloy N. This is quite significant, since the iron content of titanium-modified Hastelloy N is negligible. Thus D, or in reality a rate constant K1, is independent of the concentration of chromium, iron, and other diffusing species. The weight change, however, is quite sensitive to the total concentration of the migrating elements. Confirmation of this hypothesis is evident when K is compared with D in Hastelloy N. "3 2 For loops NCL-13 and 1 Cr 31W. R. Grimes, G. M. Watson, J. H. DeVan, and R. B. Evans, "Radi.otracer Techniques in the Study of Corrosion by Molten Fluorides," pp. 559-74 in Conference on the Use of Radioisotopes in the Physical Sciences and Industry, September 6-1 7, 1960, Proceedings, Vol 111, International Atomic Energy Agency, Vienna, 1962.
32R. B. Evans 111, J. H. DeVan, and G. M. Watson, Self-Diffusion of Chromium in Nickel-Base AZZoys, ORNL-2982 (January 1961).
71 Table 14. Rate Expressions for Material Deposited from Coolant Salt NaBF4-8 mole % NaF Oxide Content Temperaof Salt (PPm)
Weight Change Constantsa
Ti-modif ied Hastelloy N
Standard Hastelloy N
Ti-modified Hastelloy N
9 x io-’
aConstants for equation W = atb; where W = weight change, mg/cm2; t = time, hr. dW bConstants for equation dt A exp(+Q/RT)
NCL-14 at 607OC K1 = 5
cm*/sec,’while the literature value for
at 607°C is 5 x DCr constants are Do = 6.068
The appropriate Arrhenius relation
lo-’ cm2/sec and Q = 41.48 kcal/mole.
The effect of impurity oxide content in fluoroborate salt on weight losses of the Hastelloy N alloys at 555 and 604OC is given in Fig. 42. The data show that titanium-modified alloys lose less weight than the standard Hastelloy N for exposure in fluoroborate salt containing 500 ppm H20 impurity at temperatures between 555 and 604OC.
the same temperatures the titanium-modified alloy exposed to fluoroborate salt containing 1500 ppm oxide shows a greater weight loss than either alloy exposed to the 500 ppm oxide salt. The actual average weight loss rate was calculated for several
alloy-salt combinations and plotted in Fig. 43 against the inverse of the absolute temperature. rates calculated from
Also included in Fig. 43 are weight loss
STANDARD HASTELLOY N 4500ppm OXIDE IN SALT
-500 ppm OXIDE IN SALT 0 -.1.
5 TIME (hr)
Fig. 42. Weight Loss for Hastelloy N Alloys in Sodium Fluoroborate Coolant Salts. W = ( C o- Cs) J G E E , where! W = weight loss in milligrams per square centimeter of surface area, D = the diffusion coefficient in square centimeters per second, t = time in seconds, Cs and Co = the concentration maintained at surface and the initial uniform concentration, respectively, in milligrams per cubic centimeter.
73 ORNL-DWG 69- 762R2 8
A A 0 4 x
+ A 4 A 0
TYPE 304L STAINLESS STEEL Ti-MODIFIED HASTELLOY N STANDARD HASTELLOY N CALCULATED-ALLOY CONTAINS 7% Cr CALCULATED-ALLOY CONTAINS WT0 Cr FUEL SALT FLUOROBORATE COOLANT SALT TEMPERATURE ("C) 650 600
700 1 ,
I I '
5 50 1
For this calculation we assumed Cs = 0, that all weight loss was the removal of chromium, and that this removal was controlled by the diffusion of chromium to the surface. The chromium diffusion coefficient in Hastelloy N was used in the calculation. An extrapolation of the graphs of Fig. 43 shows that both fluoroborate salts (500 and 1500 ppm oxide impurity) are more aggressive than the fuel salt to the Hastelloy N alloys. Also, it appears that Adentical rates would be found â‚Źor the type 304L stainless steel-fuel salt combination and the titanium-modified Hastelloy N- fluoroborate salt (500 ppm oxide impurity).
It would be expected, if the solid-state diffusion mechanism controlled, that the calculated rates of Fig. 43 based on diffusion coefficients would be identical to the experimental rates. However, results of only the titanium-modified Hastelloy N+uel salt system coincided with the calculated values. Incidentally, fuel salts were used in the earlier experiments that showed that the rate was controlled by the diffusion coefficient of chromium in the Thus, we have shown that another mechanism besides chromium solid-state diffusion is controlling the process for several of the metal-salt systems investigated here. The weight losses of the specrmens exposed to the fluoroborate salt and the value calculated for 6OOOC and 4000 hr are compared in Table 15. It is noted that the experimental losses are greater than those calculated. As has been discussed earlier, the impurities in the fluoroborate salt appear to be very important because of the formation of HF, which is strongly oxidizing and will attack all the constituents of the Hastelloy N alloys. However, in the salt containing 500 ppm oxide impurity the titanium-modified alloy showed smaller weight losses than the standard alloy, again because of its lack of iron. In the salt with 1500 ppm oxide impurity more HF was available for attack, and the weight losses were higher, since measurable amounts of nickel and molybdenum were removed from the alloy. An increase in nickel and molybdenum concentrations is often noted in the salt analyses under these conditions. The amount of attack is approximately doubled. Because of the large amounts of nickel and molybdenum in-thealloys very little differences in the weight losses of the standard and titanium-modified alloys will be noted when large amounts of HF are available for attack. It is also believed that this HF attack is responsible for the mixed kinetics noted earlier. 33W. R. Grimes, G . M. Watson, J. H. DeVan, and R. B. Evans, "Radiotracer Techniques in the Study of Corrosion by Molten Fluorides," pp. 559-74 in Conference on the Use of Radioisotopes i n the PhysicaZ Scielices and Industry, September 6-1 7 , 1960, Proceedings, Vol 111, International Atomic Energy Agency, Vienna, 1962.
$Table’15. Effect of Impurities on Hastelloy N Corrosion by Fluoroborate Coolant Salt for 4000 hr at 600°C
Ti-modified Hastelloy N Standard Hastelloy N
Ti-modif ied Hastelloy N Calculated using D~~ = 2.0 x IO-’’ cm2/sec and C, = 0.07
0.2 ’ 1 L
With respect to the deposition process, it is obvious that the calculated rate includes only the weight changes that occur from the deposition on the surface. The amount of the diffusion into the metal
is not measured.
However, during the straight-line portion of deposition
with time, on which the kinetic calculations are based, it was theorized that the rate at which the metal deposited is the same as the rate at which it diffuses into the container wall. In time the weight gains would continue, the amount of deposited material on the surface would
remain essentially constant, and a chromium gradient would appear in the colder sections. All experimental findings do support these suppositions. The kinetic calculations for the weight-gain portion of the mass transfer show a mixed control between solid-state diffusion and solution rate. Analogous to the behavior in the hot leg, in the cold leg the weight -gains could be first solution-rate controlled and later, as the process slows down, be controlled by the diffusion. Thus, the overall 4
effect would be mixed control. As theorized earlier it still appears that the action in the cold leg controls the mass transfer process for I
the entire system. In liquid metal systems, the simple approach to the mass transfer problem is the statement that the weight ,loss rate is a function of the
difference in the solubility of the dissolved metal at the temperatures
of interest.' The proportionality constant may be related to the diffusion coefficient of the metal in the liquid if diffusion is the controlling step or may be related to another factor concerning some process occurring at the inteeface if the rate of solution is controlling. However, many additional models have been required to explain all the experimental findings. The most ticklish problems involve the possible effect of oxygen on the solubility of certain metals in liquid metals, the velocity effect, and the downstream effect. Similar problems exist in the fused fluoride salt systems. In the salt systems, we can make the general statement that the corrosion rate in fuel salts is a function of the chromium and iron contents of the alloy. In the fluoroborate salts, the rate is a function of the alloy composition and the impurity level of the salt. The proportionality constant for both cases is a function of temperature and can be found experimentally. As in liquid metal systems, the rate controlling mechanisms are not entirely clear cut but are functions of many variables. Although the corrosion of these systems has been widely discussed, it should be pointed out that the weight loss rates are quite low. SUMMARY
Our data on mass transfer in the fluoroborate salt mixture points out that impurities such as water and oxygen strongly affect the fluoride oxidation potential of this salt. However, we do not yet completely know the chemical forms taken by these impurities upon entering the salt. Corrosion rates show a marked increase following an air or steam.leak into the fluoroborate salt. Once the leak has been detected and corrected, the corrosion rate drops sharply. Analyses of the salt shows an increase in oxide level as the corrosion rate increases; the explanation for this behavior is that moisture reacts with the salt to produce HF and compounds (oxides and hydroxides) that analyze as oxides by the present techniques. The HF causes rapid oxidation of the containment material and is used up in the process.
The compounds that analyze as water and oxygen remain
but have only a minor effect on corrosion rate. Kinetic considerations showed that the mass transfer process is between solid-state diffusion
control and solution control, probably depending on the amount of impurities.allowed to enter the salt. The mass transfer behavior is very similar to that seen for the chromium-ZTF4 corrosion reaction, the difference being that other alloy constituents (beside chromium) participate in the process and the reaction rates are different. We have also shown the difficulty.in keeping the fluoroborate salt mixture free. of moisture-type impurities but feel that this can be done by exercising sufficient care. Except for certain periods of the fluoroborate tests, the overall corrosion rates have been relatively small. Thermal-convection loop NCL-14 has 'operated successfully for over two years and the pump loop MSR-FCL-1 nearly one year with the fluoroborate mixture. Comparison of the rates experienced by NCL-13A, NCL-14, and MSR-FCL-1, all circulating the sodium fluoroborate mixture, indicates a velocity effect on the mass transfer (Table 16). We believe that the effect of velocity on corrosion in this system is a function of declining importance as the purity level
of the salt improves. The impurity effect per se has been discussed in detail previously. Because of the importance of the impurities on the corrosion of Hastelloy N by fluoroborate, efforts have begun on methods of purifying the salt. Also to be considered are better methods for analyzing and identifying the impurities. At some purity Level, perhaps 200 to 400 ppm oxide as analyzed, solid-state diffusion of chromium in the Hastelloy N will likely control corrosion, as it does in the fuel salts. This is most important, since it suggests that an entire MSBR of either the one- or two-fluid variety can be operated with none of the e than a few tenths of a mil per main circulating channels suffering year corrosion attack. Experimental proof of this is one of our major near-term goals,
78 Table 16. Comparison of Corrosion Rates for Standard Hastelloy N in MSR Systems After More Than 5000 hr Operation
MSR-FCL-1 NCL-16 NCL-15A
Maximum Temperature Temperature Difference ("0 ("C)
605 605 588 705 675 705
Equivalent Corrosion Rate (fps) (mils/year)
0.1 10 0.1 0.1 0.1
0.6 0.55 1.2 0.04 0.03 0.05
(92-8 mole %j,1000 ppm oxide. 200 ppm oxide. bLiF-BeF,4JF4 (65.5-34.0-0.5 mole %), CLiF-BeFz-ThF, (73-2-25 mole %), < 200 ppm oxide. dLiF-BeF2-ThF~-UF~ (68-20-11.7-0.3 mole %) , < 200 ppm oxide. aNaBF,+aF
1. The corrosion rate is a function of the alloy composition and impurity level of the salt. 2. Because of the corrosive nature of the BF3 in an impure state and because it is present in appreciable quantities over the melt, leaks in mechanical portions of the systems can easily occur. 3. Kinetic considerations disclose that the weight change rates are controlled by a mixture of solid-state diffusion and solution rate. 4. The effective diffusion rate that controls the hot-leg attack is larger than the volume diffusion coefficients obtained in typical diffusion experiments. 5. The mass transfer behavior (weight losses in hot leg, weight gains in cold leg, steady balance points) is very similar to that seen for the chromium-UF, corrosion reaction.
Titanium-modified Hastelloy N with less chromium and iron shows a greater resistance to attack in a fluoroborate salt with 500 ppm oxide
impurity than standard Hastelloy N. The corrosion rate of titanium-modified Hastelloy N in fluoroborate salt with 1500 ppm oxide impurity is double that found in'salt with 500 ppm oxide.
Corrosion rates were relatively low for all systems tested. ACKNOWLEDGMENT
It is a pleasure to acknowledge that E. J. Lawrence supervised construction and operation of ,the thermal convection loops and was responsible for the weight change measurements of all the corrosion specimens. We also recognize P. A. Gnadt and W. R. Huntley of the Reactor Division for operation and design of the pump loop. We thank A. P. Litman for his invaluable assistance through part of this work. f
We are also indebted to H. E. McCoy, Jr., J. H. Devan, T. S. Lundy, and J. V. Cathcart for constructive review of the manuscript. Special.thanks are extended to the Metallography group, especially H. R. Gaddis, C. E. Zachery, H. V. Mateer, T. J. Henson, and R. S. Crouse and to the Analytical Chemistry Division, particularly Cyrus Feldman and H. W. Dunn, the Graphic Arts Department, the Metals and Ceramics Division Reports Office, and particularly S. Peterson, for invaluable assistance.
81 0RNL-~hi-38 66 INTERNAL DISTRIBUTION (113 copies) (3) Central Research Library ORNL - Y-12 Technical Library Document Reference Section (10) Laboratory Records Department Laboratory Records, ORNL RC ORNL Patent Office (2) MSRP Director's Office (fi-12) G. M. Adamson, Jr. J. L. Anderson R. F. Apple C. F. Baes S. E. Beall E. S. Bettis F. F. Blankenship E. G. Bohlmann G. E. Boyd R. B. Briggs S . Cantor J. V. Cathcart 0 . B. Cavin N. C. Cole R. S. Crouse J. L. Crowley F. L. Culler 3. E. Cunningham J. M. Dale J. H. DeVan J. R. DiStefano S. J. Ditto H. W. Dunn P . Eatherly
W. J. C. D.
R. Engel Feldman E. Ferguson
R. T. (3) M. W. H. P. J. (10) J. A.
. J.I. Lundin Lawrence
M. T. R. D. W. H. H. C. B. L. A. R. F. E. P. A. C.
H Frye, Jr. R. Gaddis 0 . Gilpatrick A. Gnadt J. Gray R. Grimes G. Grindell R. H. Guymon w. 0 . Harms P. N. Haubenreich
Sc. Lundy E. MacPherson L. Manning R. Martin V. Mateer E- McCoy, Jr, J. McHargue McNabb E. McNeese S. Meyer L. Moore H. Neil1 L. Nicholson Patriarca M. Perry B. Pollock
H. C. Savage
D. J. J. G.
D. R. J. H. L. P. R. W. A.
E. Helms J. Henson R. Hill R. Huntley Inouye R. Kasten J. Keyes W. Koger I. Krakoviak
D. G. A.
J. M, J. G. J. C.
ScottL; Scott H. Shaffer M. Slaughter Sood E. Thoma B. Trauger M. Watson M. Weinberg R. Weir, Jr. E. Whatley C. White Young P. Young E. Zachary
(38 copies) AEC DIVISION OF REACTOR DEVELOPMENT AND TECHNOLOGY, Washington, DC 20545 A. J. N. ( 2 ) T.
R. DeGrazia E. Fox Haberman W. McIntosh J. F. Neff M. Shaw
AEC DIVISION OF REACTOR,LICENSING,Washington, DC 20545 (3) P. A. Morris AEC DIVISION OF REACTOR STANDARDS, Washington, DC 20545 ( 2 ) E. G. Case
AEC DIVISION OF SPACE NUCLEAR SYSTEMS, Washington, DC 20545 A. P. Litman AEC MSBR PROGRAM, Washington, DC 20545 ( 2 ) Program Manager AEC OAK RIDGE OPERATIONS, P. 0 . Box E, Oak Ridge, TN 37830 Research and Technical Support Division AEC-RDT SITE REPRESENTATIVES, Oak Ridge National Laboratory, P. Oak Ridge, TN 37830
D. F. Cope K. Laughon TECHNICAL INFORMATION CENTER, Office of Information Services, P. 0 . Box 6 2 , Oak Ridge, TN 37830 ( 2 ) Manager (17) Manager (for transmittal to members of ACRS) UNIVERSITY OF TENNESSEE, Department of Nuclear Engineering, Knoxville, TN 37916
H. G. MacPherson